Revista de la Asociación Latinoamericana de Control de Calidad, Patología y Recuperación de la Construcción

## Revista ALCONPAT

www.revistaalconpat.org eISSN 2007-6835

**Influence of anchorage on flexural strength of beams strengthened with CFRP **

**sheets **

M. P. Ferreira 1_{* } _{, M. H. Oliveira}2 _{ A. F. Lima Neto}3 _{, L. S. Tapajós}4 _{, }

A. J. C. Nascimento5 , M. C. Freire3

*Contact author: mpinaf@gmail.com DOI: http://dx.doi.org/10.21041/ra.v9i1.269

Reception: 29/09/2017 | Acceptance: 18/10/2018 | Publication: 30/12/2018

**ABSTRACT **

In order to evaluate the influence of anchorage on the flexural strength of beams strengthened with Carbon Fiber Reinforced Polymer (CFRP) sheets, the experimental results of 126 tests in the literature and of an unprecedented series with 4 reinforced concrete beams, tested by these authors, were analyzed. The parameters affecting the performance and the strength of the beams are evaluated, and the design criteria of fib Bulletin 14 (2001) and ACI 440-2R (2008) are discussed. It was observed that, even with auxiliary devices in the PRFC anchorage, premature failure is possible, and that both theoretical recommendations lead to safe estimates, but excessively conservative in cases where the anchorage of the PRFC sheet is properly done.

**Keywords: **reinforced concrete; flexural strengthening; CFRP sheets; anchorage.

_______________________________________________________________
1 _{Civil Engineering Department, Federal University of Pará, Belém, Brazil.}

2 _{Civil and Environmental Engineering Department, University of Brasília, Brasília, Brazil.}
3 _{Nucleus of Amazonian Development in Engineering, Federal University of Pará, Tucuruí, Brazil.}
4 _{Civil Engineering Department, Federal University of the West of Pará, Itaituba, Brazil }

5 _{Post-graduation in Civil Engineering, Federal University of Pará, Belém, Brazil. }

**Legal Information **

Revista ALCONPAT is a quarterly publication by the Asociación Latinoamericana de Control de Calidad, Patología y Recuperación de la Construcción, Internacional, A.C., Km. 6 antigua carretera a Progreso, Mérida, Yucatán, 97310, Tel.5219997385893,

alconpat.int@gmail.com, Website: www.alconpat.org

Responsible editor: Pedro Castro Borges, Ph.D. Reservation of rights for exclusive use No.04-2013-011717330300-203, and ISSN 2007-6835, both granted by the Instituto Nacional de Derecho de Autor. Responsible for the last update of this issue, Informatics Unit ALCONPAT, Elizabeth Sabido Maldonado, Km. 6, antigua carretera a Progreso, Mérida, Yucatán, C.P. 97310.

The views of the authors do not necessarily reflect the position of the editor.

The total or partial reproduction of the contents and images of the publication is strictly prohibited without the previous authorization of ALCONPAT Internacional A.C.

Any dispute, including the replies of the authors, will be published in the third issue of 2019 provided that the information is received before the closing of the second issue of 2019.

Revista ALCONPAT, 9 (1), 2019: 30 – 47

**Influência da ancoragem na resistência à flexão de vigas reforçadas com **

**mantas de PRFC **

**RESUMO **

Buscando avaliar a influência da ancoragem na resistência à flexão de vigas reforçadas com mantas de Polímero Reforçado com Fibra de Carbono (PRFC), foram analisados os resultados experimentais de 126 ensaios presentes na literatura e de uma série inédita, ensaiada pelos autores, com 4 vigas de concreto armado. São avaliados os parâmetros que afetam o desempenho e a resistência das vigas, e discutidos os critérios de dimensionamento do fib Bulletin 14 (2001) e ACI 440-2R (2008). Observou-se que, mesmo com dispositivos auxiliares na ancoragem do PRFC, falhas prematuras são possíveis, e também que ambas as recomendações teóricas conduzem a estimativas a favor da segurança, porém excessivamente conservadoras nos casos onde a ancoragem da manta de PRFC é feita adequadamente.

**Palavras-chave:** concreto armado; reforço à flexão; mantas de PRFC; ancoragem.

**Influencia del anclaje en la resistencia a la flexión de vigas reforzadas con **

**mantas de PRFC **

**RESUMEN **

Buscando evaluar la influencia del anclaje en la resistencia a la flexión de vigas reforzadas con mantas de Polímero Reforzado con Fibra de Carbono (PRFC), se analizaron los resultados experimentales de 126 ensayos presentes en la literatura y de una serie inédita de los autores, con 4 vigas de hormigón armado. Se evalúan los parámetros que afectan desempeño y resistencia de vigas, y se discuten los criterios de dimensionamiento del fib Bulletin 14 (2001) y ACI 440-2R (2008). Se observó que, incluso con dispositivos auxiliares en el anclaje del PRFC, fallos prematuros son posibles, y que ambas recomendaciones conducen a estimaciones seguras, pero excesivamente conservadoras en los casos en que el anclaje de la manta de PRFC se realice adecuadamente.

**Palabras clave:** hormigón armado; refuerzo de la flexión; mantas de PRFC; fondeadero.

**NOMENCLATURE **

*a * – shear span

*b*f – width of the layer of CFRP

*b*w – width of the beam

*c * – height of the block of rectangular
compression equivalent of the
concrete

*c*1 – factor obtained by calibration of

results (equal to 0.64 for CFRP)
*d * – effective beam height

*d’ * – centroid position of the compressed
reinforcement

*f*c – concrete compression strength

*f*ctm – average tensile strength of concrete

*f*fe – effective strength of the CFRP

*f*s – strength in the steel of the tensile

reinforcement

*f*s’ – steel strength of the compressed

reinforcement

*f*ys – yield strength of the tensile

reinforcement

*f*ys’ – yield strength of the compressed

reinforcement
*h * – height of the beam
*k*b – geometric factor

*k*c – constant that considers the

compacting of the concrete during the concreting

*lb* – anchoring length of the CFRP sheet

*l * – clamping width

*n * – number of layers of CFRP
*t*f – thickness of the CFRP

Revista ALCONPAT, 9 (1), 2019: 30 – 47

Af – area of reinforcement applied to the beam

As – steel area of the tensile reinforcement

As’ – steel area of compressed reinforcement

*C*C – compression component due to the

concrete portion

*C*S – compression component due to

compressed reinforcement

*E*f – modulus of elasticity of the CFRP

*E*s – modulus of elasticity of steel

*F*cc – compression resulting

*L * – total beam length

*M * – moment applied during the
experimental test

*M*R – resistant moment in the cross

section of the beam

*M*Rteo – resistant moment estimated by the

recommendations

*M*u – experimental ultimate moment

*M*ACI – ultimate moment according to the

recommendations of ACI 440-2R (2008)

*Mfib* – ultimate moment according to the

recommedations of fib Bulletin 14 (2001)

*M*V1 – experimental ultimate moment of

the beam V1

*N*fa,max – maximum force that can be applied

to the reinforcement of the beam
*P * – applied load in the experimental

test

R² – coefficient of correlation of the results

*T*f – tensile component due to the fiber

reinforcement portion

*T*s – tensile component due to the tensile

reinforcement

α – reduction coefficient due to the propagation of inclined cracks β1 – coefficient that determines the

approximation of the resultant compression curve of the concrete to a rectangle according to the

recommendations of ACI 440-2R (2008)

*ε*bi – strain found in the covering of the

tensile reinforcement in the beam before the strengthen

*ε*c – concrete strain

*ε*cu – concrete ultimate strain

*ε*f – carbon fiber strain

*ε*fd – limit value of fiber strain to be

adopted in the sizing and verification of reinforcement

*ε*fe – effective strain in the CFRP

*ε*fu – ultimate strain observed in the

polymer at the moment of failure
*ε*s – strain in the tensile reinforcement

*ε*s’ – strain in the compressed

reinforcement

*ε*ys – yield strain of the flexural

reinforcement

r – rate of the reinforcement of the beam before the strengthen rr – beam reinforcement ratio after

strengthen

∅ – reinforcement bar diameter ψ – coefficient that determines the

approximation of the resulting curve of concrete compression to a rectangle, according to the recommendations of fib Bulletin 14 (2001)

**1.**

**INTRODUCTION **

Revista ALCONPAT, 9 (1), 2019: 30 – 47

However, it is important to feature that premature failures are associated with its use. In the case of flexural reinforced beams, this brittle fracture may occur due to the detachment of the carbon fiber from the concrete substrate, which may limit the increase in strength provided by the reinforcement. This mode of brittle ruin is usually associated with deficiency in the anchorage of the reinforcement system, which makes the use of additional devices recommended, such as band clipping of CFRP sheet (see Benjeddou et al., 2007; Dong et al., 2011, Kim and Shin, 2011, among others).

This work presents a series of experimental tests on reinforced concrete beams strengthened with CFRP sheets, carried out with the objective of evaluating the influence of the anchorage in the reinforcement structural performance. In addition, a large database was set up, with experimental results selected from the work of different authors. This database is used to discuss the influence of different parameters on the performance of reinforcement with CFRP sheets and to evaluate the performance of theoretical predictions of strength obtained using the recommendations presented by ACI 440-2R (2008) and fib Bulletin 14 (2001).

**2.**

**CFRP STRENGTHENED BEAMS **

**2.1 Failure modes **

Teng et al. (2003) state that beams strengthened to flexure with CFRP sheets may exhibit brittle failure modes, for instance: by exhaustion of the strength of the CFRP (see Figure 1a); detachment of the reinforcement at the interface with the concrete (see Figure 1b); and separation of the reinforcement together with the concrete covering of the flexural reinforcement (see Figure 3c). The failure of the CFRP sheet can occur in weakly reinforced beams by flexure, being a brittle mode of failure since the CFRP presents linear-elastic behavior until the failure. The detachment of the sheet may occur due to lack of the anchorage of reinforcement, excessive cracking of the beam or, faults in its bonding process. The separation of concrete cover layer can be caused by shear strengths at the interface between concrete and CFRP due to the difference between the moduli of elasticity of these materials, which can be amplified by the corrosion of the bending reinforcement.

a) Failure b) Detachment c) Separation

Figure 1. Failure modes of beams strengthened to flexure with CFRP.

**2.2 ** **Flexural Strength **

Revista ALCONPAT, 9 (1), 2019: 30 – 47

Figure 2. Stress-strain diagram of a beam strengthened with CFRP.

*f*
*r*
*s*
*w*
*f*
*E*
*A*

*b* *h E*

+ = (1)

Where: ρ is the rate of the reinforcement of the beam before the strengthening; Af is the area of

reinforcement applied to the beam; Ef is the modulus of elasticity of the CFRP; Es is the modulus

of elasticity of steel; bw is the width of the beam; h is the height of the beam.

**2.2.1 ACI 440-2R (2008) **

The American code ACI 440-2R (2008) presents recommendations for the sizing of reinforcement using CFRP. To determine the flexural strength of reinforced concrete beams reinforced with carbon fiber sheets, (2) - (10) are used.

0, 41 *c* 0, 9

*fd* *fu*

*f* *f*

*f*

*n E* *t*

=

(2)

*fe* *cu* *bi* *fd*

*h* *x*

*x*

= _{} − _{}−

(3)

*fe* *f* *fe*

*f* =*E*

###

(4)'
'
*s* *cu*
*x* *d*
*x*
= _{} − _{}
(5)
*s* *fe*
*d* *x*
*h* *x*
= _{} − _{}
−
(6)
' ' '

*s* *s* *s* *ys*

*f* = *E*

###

*f*(7)

*s* *s* *s* *ys*

*f* =*E* *f* (8)

1

( ) ( ) ( ' ')

0,85

*s* *s* *f* *fe* *s* *s*

*c* *w*

*A* *f* *A* *f* *A* *f*

*x*
*f b*
+ −
=
(9)
*x*
L.N.
Afibra
*x*
*A _{S'}*

*A*

_{S}*Fcc*

*Ts* *Ts*

*C _{S}*

*C _{C}*

*0,85.fc*

###

*c*

### '

s###

s*T*_{f} *T*_{f}

###

_{f}

*c*

*A*_{f}

*bw*

*d'*

Revista ALCONPAT, 9 (1), 2019: 30 – 47

1 1 1

0,85 ' ' '

2 2 2

*R* *s* *s* *f* *fe* *s* *s*

*x* *x* *x*

*M* = *A* *f* _{}*d*− _{}+ *A* *f* _{}*h*− _{}+*A* *f* _{} −*d* _{}

(10)

Where: εfd is the limit value of fiber strain to be adopted in the sizing and verification of

reinforcement to avoid premature fiber failure; n is the number of layers of CFRP; tf is the thickness

of the CFRP; εfu is the ultimate strain observed in the polymer at the moment of failure; εfe is the

effective strain in the CFRP; x is the position of the neutral axis; εbi is the strain found in the

covering of the tensile reinforcement in the beam before the strengthen; ffe is the effective strength

of the CFRP; d is the effective beam height; εs' is the strain in the compressed reinforcement; fs' is

the strength in the steel of the compressed reinforcement; d’ is the centroid position of the compressed reinforcement; εs is the strain in the tensile reinforcement; fs is the strength in the steel

of the tensile reinforcement; As is the steel area of the tensile reinforcement; As' is the steel area of

compressed reinforcement; β1 is a coefficient that determines the approximation of the resultant

compression curve of the concrete to a rectangle, being 0.85 for concrete with fc values lower than

28 MPa and there being a linear decrease of 0.05 for each 7 MPa above that limit of strength, the minimum value for such a coefficient, according to ACI 318 (2014), is 0.65; MR is the tough moment in the cross section of the beam.

**2.2.2 fib Bulletin 14 (2001) **

The fib Bulletin 14 (2001) presents recommendations for the dimensioning of flexural reinforced beams with CFRP and adopts a calculation philosophy like that adopted by ACI 440-2R (2008). The same equations presented by the ACI are used in this document, differentiating only the following parameters: the coefficient β1 in it is called of ψ and equals to 0.8, independent of the class of strength of the concrete; and the strain limit of the fiber, which is calculated by (11), whose parameters are found by means of (12) - (14).

,

*fa max*
*fd*

*f* *f*

*N*

*E* *A*

=

(11)

, 1

*fa max* *c* *b* *w* *f* *f* *ctm*

*N* = *c k k b* *E* *t* *f*

(12)

2

1, 06 1

1 400

*f*

*w*
*b*

*f*

*b*

*b*
*k*

*b*
−

=

+ (13)

0, 33

*ctm* *c*

*f* = *f* (14)

Where: Nfa,max is the maximum force that can be applied to the reinforcement of the beam

(expressed in N); α is a reduction coefficient due to the propagation of inclined cracks, adopted as 0.9; c1 is equal to 0.64; kc is a constant that considers the compacting of the concrete during the

concreting, being this value equal to 1 when the strengthening is applied in the underside of the beam and 0.67 in the upper face; kb is a geometric factor; fctm is the average tensile strength of

Revista ALCONPAT, 9 (1), 2019: 30 – 47

**3.**

**EXPERIMENTAL PROGRAM **

**3.1 Characteristics of the beams **

Tests were carried out on 4 reinforced concrete beams strengthened with CFRP sheets, having as variables the sheet anchorage length and width in order to evaluate their influence on both the performance and the strength of the beams. It was tested 1 reference beam without reinforcement and 3 reinforced beams with carbon fiber sheet. The rates of steel reinforcement and CFRP were kept constant. Table 1 and Figure 3 show the main characteristics of the beams. The strains in the flexural reinforcement, the reinforcement sheet and the clamping were monitored with electrical extensometers, as shown in Figure 4. Figure 5 shows the test system of the beams.

Table 1. Characteristics of the tested beams.

**Beam ** **l****(mm) ** **l****b**** (mm) ****b****f**** (mm) ****A****f**** (mm²) ****t****f**** (mm) ****E****f**** (GPa) ****ε****fu**** (%) **

V1 - - - -

V2

100 285

120 19.92 0.166 230 2.1

V3

385

V4 150

*bw* = 120 mm; h = 200 mm; d = 166 mm; A*s* = 101 mm²; f*c* = 20 MPa; a = 400 mm

a) V1 b) V2

c) V3 d) V4

Figure 3. Characteristics of tested beams.

a) Flexural reinforcement b) CFRP

Revista ALCONPAT, 9 (1), 2019: 30 – 47

Figure 5. Test system of beams.

**3.2 Discussion of Results **

The failure mode of each of the beams tested can be visualized in Figure 6. It was observed that the reference beam failed by flexure after its longitudinal reinforcement reached high levels of strain (Figure 6a). In the V2 beam the concrete was pulled out in the zone adjacent to the clamping (Figure 6b). The V3 beam lost its strength after the fiber detachment occurred in part of the clamping contact zone (Figure 6c). However, the V4 beam failed after the detachment of the concrete covering in the region of the flexure span (Figure 6d).

a) V1 b) V2

c) V3 d) V4

Figure 6. Failure surface of tested beams.

Revista ALCONPAT, 9 (1), 2019: 30 – 47

both the anchoring length of the fiber and the clamping width influenced the ultimate strain of the CFRP measured in the tests, varying from 3.5 ‰ for the beam V2 to approximately 4.2 ‰ for the beams V3 and V4. In all cases, it should be noted that these values are higher than theoretically predicted by the ACI, which would be 1.9 ‰. It should be emphasized that none of the beams failed with the exhaustion of the tensile strength of the sheet of CFRP. Figure 7c shows that in all the beams the level of strain at the end of the reinforcement was smaller than that measured in the middle of the span, where the moment is maximum and that in the case of the beam V2, which failed due to the detachment of the fiber in this region, the strain limit measured was practically the same as that suggested by the manufacturer of 2.1 ‰. In Figure 7d it is possible to notice that the level of strain developed in the region of the clamping was small and that in beam V3 it clearly begins to separate before the failure.

a) Moment x Strain curve in the flexural

reinforcement

b) Moment x Strain curve of the CFRP sheet in the middle of the span

c) Moment x Strain curve of the CFRP sheet at the end of the reinforcement

d) Moment x Strain curve of the CFRP sheet in the clamping

Figure 7. Results of the beams tests.

Revista ALCONPAT, 9 (1), 2019: 30 – 47

Figure 8. Moment-displacement curves of the tested beams.

Table 2 presents the final loads of the tested beams and compares the strength of the reinforced beams with the sheet of CFRP with the reference beam (V1), in order to determine the increment of strength generated by the reinforcement. In addition, the experimental strength of the beams is compared with theoretical estimates obtained following the recommendations of the ACI and fib14. From these results, it was observed that the increase of the anchoring length of the beam V3 in relation to the beam V2 did not result in an increase of strength, and that the increase of the clamping width was responsible for the greater strength of the beam V4 in relation to the beam V3. It was also observed that the use of ACI would result in predictions of strength against safety for beams V2 and V3, while fib14 presented results in favor of safety.

Table 2. Ultimate loads of the beams.

**Beam ** **M****u ****(kN.m) ** **M****u ****/ M****V1** **M****u ****/ M****ACI** **M****u ****/ M****fib**

V1 10.2 1.00 - -

V2 13.2 1.29 0.94 1.14

V3 13.2 1.29 0.94 1.14

V4 14.6 1.43 1.04 1.26

**4.**

**DATABASE **

**4.1 Methodology of collection and analysis of data **

In addition to the experimental program, a database was collected with the results of 126 tests of 20 authors, involving flexural reinforced beams with the sheet of CFRP. As a criterion for the choice of beams, only those that failed by bending, without initial loading and externally bonded reinforcement, were selected. The objective of this data analysis is to evaluate the influence of the main variables on the flexural strength of reinforced beams with CFRP.

The analysis of the database involves the comparison of the experimental results with the
theoretical estimates obtained using the ACI and *fib 14. Thus, it was calculated the values of *
average, coefficient of variation and standard deviation of the ratio between the experimental
ultimate moment and the theoretical resistant moment (Mu/MRteo), and finally, the percentage of

safety results (Mu/MRteo <1) was evaluated. In order to evaluate the precision of the theoretical

models, graphs are presented that compare the moment of experimental failure (Mu) by the function

of the predicted resistant moment (MRteo), in order to analyze if the tendency of the obtained results

approaches the ideal condition (Mu=MRteo).

0 2 4 6 8 10 12 14 16 18 20

0 1 2 3 4 5 6 7 8 9 10 11 12

**M**

** (k**

**N**

**.m**

**)**

**Displacement (mm)**

Revista ALCONPAT, 9 (1), 2019: 30 – 47

As previously noted, the performance of the reinforcement with sheet of CFRP is directly related to the quality of fiber anchoring to concrete. Therefore, the beams of the database were divided into 3 groups: group 1 for situations where the bonding of the sheet stretched from the center of the beam to the support or beyond; the group 2 with beams in which the glue of the sheet did not extend to the support; and the group 3 with beams in which external devices were used to aid in reinforcement anchorage, such as screws or restrainers. It should be noted that this type of anchorage is considered by several authors as the most favorable for anchoring the CFRP sheet, since that the device is made of this same material.

Another method used was the Collins (2001) criterion, known as *Demerit Points Classification *
(DPC), in which the values of Mu/MRteo were classified in ranges from "extremely dangerous" to

"extremely conservative", with performance of the theoretical model defined as a number resulting
from the sum of the products from *M*u/MRteo by their corresponding score, according to the

classification. Table 3 presents a summary of the characteristics of the beams of the database, as well as the symbology used by the authors to identify the figures. Table 4 shows a summary of the variables related to the reinforcement with carbon fiber sheet of the beams of the database. Table 5 presents the parameters related to Collins DPC (2001).

Finally, were prepared graphs which relate the experimental strength of the beams to the predicted theoretical failure (Mu/MRteo) according to the number of layers of CFRP sheets, as well as the

reinforcement ratio after strengthening in relation to the initial reinforcement (ρr/ρ). The purpose

of these charts is to analyze if the hypotheses adopted by the theoretical models present adequate correlation with the existing experimental evidence.

Table 3. Characteristics of the database beams.

**Author ** **No. of **

**beams **

**b****w**

**(mm) **

**h ****(mm) **

**d ****(mm) **

**a ****(mm) **

**A****s**

**(mm²) **
**f****ys****(MPa) **

**f****c****(MPa) **

Beber (2003) 12 150 300 272 833 245 706 32

Beber *et al.* (2000) 8 120 250 219 783 157 565 33
David *et al.* (2003) 4 150 300 267 933 307 500 39
Esfahani *et al. *

(2007) 6 150 200 164 600 402-626 350-406 24

Breña *et al.*(2003) 9 203 356-406 318-368 1065-1220 395 440 35-37
Rusinowski *et al.*(2009) 5 200 300 262 1300 402 527 64-70
Toutanji *et al.*

(2006) 7 108 158 127 560 142 427 49

Barros *et al.* (2007) 6 120 170 141-145 300 39-99 627-788 44

Gamino (2007) 14 75 150 120 550 62 640 45

Zhang *et al.* (2006) 4 120 250 224 750 226-402 335 23
Spadea *et al.* (2000) 2 140 300 266 1800 402 435 30
Alagusundaramoothy *et *

*al.*(2003) 12 230 380 342 1830 981.75 414 31

Ferrari (2007) 3 170 350 300 950 254.4 548 35-38

Dias *et al. *(2002) 5 120 180 160 720 100.5 533 41
Balaguru e Kurtz

(2001) 3 200 300 255 1000 258 447 47

Vieira *et al. *(2016) 8 120 245 220 800 157-245 500 44
Bilotta *et al. *(2015) 2 120 160 135 925 157 590 21

Garcez (2007) 2 150 300 270 950 245.4 578 41.4

Juvandes (1999) X 9 75-150 150 130 605-650 14-226 192-507 20-45 Chahrour e Soudki

Revista ALCONPAT, 9 (1), 2019: 30 – 47

Table 4. Strengthening variables of the beams.

**Author ** **No. of **

**beams **

**No. of **
**layers **

**b****f ****(mm)**

**t****f ****(mm) **

**A****f ****(mm²) **

**E****f ****(GPa) **

**e****fu ****(‰) **

Beber (2003) 12 1-6 50-150 0.1-1.4 10-140 240 12-14

Beber *et al.* (2000) 8 1-10 120 0.011 1.3-13.2 230 15

David *et al.* (2003) 4 2-4 50 1.2 120-240 150 15

Esfahani *et al. *(2007) 6 1-2 100-150 0.176 17.6-52.8 237 12
Breña *et al.*(2003) 9 1-2 50-100 0.165-1.2 16.5-104 62-230 12-16
Rusinowski *et al.* (2009) 5 1-2 50-120 1.4 140-168 155-300 9-15
Toutanji *et al.* (2006) 7 3-6 102 0.165 50.5-101 110 6
Barros *et al.* (2007) 6 1-3 9.6-80 0.1-1.4 13.4-40.3 158.8-240 15-17
Gamino (2007) 14 1-2 75 0.11-0.13 8.2-16.5 230-235 15
Zhang *et al.* (2006) 4 1-2 120 0.11 13.3-26.6 235 14.27

Spadea *et al.* (2000) 2 1 80 1.2 96 152 15.1

Alagusundaramoothy *et al. *

(2003) 12 1-3 76-203 1.4-4.7 36.4-975 48-228 11.5-15

Ferrari (2007) 3 1-3 16.5 0.17 2.8-8.4 50 13

Dias *et al. *(2002) 5 1-2 20-70 0.1-1.4 15.5-28 200-240 11-15
Balaguru e Kurtz (2001) 3 2-5 152 0.071 21.6-54 200 6
Vieira *et al. *(2016) 8 2-5 100 0.166 33.2-83 230 21

Bilotta *et al. *(2015) 2 1-2 40 1.4 56-112 171 12

Garcez (2007) 2 1-2 150 0.165 247-49 227 15

Juvandes (1999) 9 1 50 1.2 60 155 19

Chahrour e Soudki (2005) 5 1 100 1.2 120 155 19

Table 5. Collins criterion.

**M****exp/MRteo ** **Classification ** **Penalty **

< 0.50 Extremely Dangerous 10

(0.50 - 0.65) Dangerous 5

(0.65 - 0.85) Low Safety 2

(0.85 -1.15) Proper Safety 0

(1.15 - 2.00) Conservative 1

≥ 2.00 Extremely Conservative 2

**4.2 Discussion of Results **

Revista ALCONPAT, 9 (1), 2019: 30 – 47

a) ACI 440-2R (2008)

b) *fib Bulletin 14 (2001) *

Figure 9. Analysis of the theoretical model’s accuracy.

In order to evaluate the influence of the type of anchorage of the reinforcement with CFRP in the
performance of the theoretical predictions, Figure 10 divides the general data presented in Figure
9, classifying them by type of anchorage in 3 distinct groups. For group 1, ACI presented an
average closer to 1.0, as well as a lower dispersion of results and approximately the same number
of values against safety, when compared with fib 14. In group 2, this behavior was reversed, and
*fib 14 showed lower average, but still with greater dispersion and greater percentage of results *
against the safety. For the beams of group 3 the theoretical methods presented similar performance,
with the ACI showing again less dispersion.

As seen, using Collins criterion (2001), it is possible to establish scores for the two recommendations, based on the sample space of the collected database, as shown in Figure 11. It is observed that the ACI presents a lower penalty according to the criterion adopted.

y = 1.3414x R² = 0.9301

0 30 60 90 120 150

0 30 60 90 120 150

M

u (

kN

.m)

MACI (kN.m) MÉD.: 1,18 D.P.: 0,27 C.V.: 23,1% R.C.S.: 24,0%

y = 1.3414x R² = 0.9301

100 150 200 250 300

100 150 200 250 300

M

u (

kN

.m)

MACI (kN.m) MÉD.: 1,18 D.P.: 0,27 C.V.: 23,1% R.C.S.: 24,0%

y = 1.2156x R² = 0.9108

0 30 60 90 120 150

0 30 60 90 120 150

M

u (

kN

.m)

Mfib14 (kN.m) MÉD.: 1,17 D.P.: 0,31 C.V.: 26,7% R.C.S.: 31,8%

y = 1.2156x R² = 0.9108

100 150 200 250 300

100 150 200 250 300

M

u (

kN

.m)

Revista ALCONPAT, 9 (1), 2019: 30 – 47

a) ACI – Group 1 b) ACI – Group 2 c) ACI – Group 3

d) *fib – Group 1 * e) *fib – Group 2 * f) *fib – Group 3 *

Figure 10. Analysis of the theoretical models accuracy in relation to the anchorage type.

a) Collins penalties b) Distribution of beams results

Figure 11. Result of the Collins criterion (2001).

Figure 12 analyzes the influence of the number of layers of CFRP on both reinforcement performance and theoretical methods. It is noticed that there is a trend of more conservative results as the amount of layers increases, which is justified by the fact that both recommendations limit the strain of CFRP. For the ACI, this trend is slightly higher, since in its equation the number of layers is used, which penalizes the strength estimation of reinforced beams with a high number of layers. In contrast, in fib 14 this factor is not considered.

y = 1.1399x R² = 0.9713

0 20 40 60 80 100

0 20 40 60 80 100

M u ( kN .m) MACI (kN.m) MÉD.: 1,13 D.P.: 0,17 C.V.: 15,0% R.C.S.: 25,0%

y = 1.3749x R² = 0.9073

0 50 100 150 200 250 300

0 50 100 150 200 250 300

M u ( kN .m) MACI (kN.m) MÉD.: 1,27 D.P.: 0,33 C.V.: 26,1% R.C.S.:17,1%

y = 0.9636x R² = 0.9609

0 20 40 60 80 100

0 20 40 60 80 100

M u ( kN .m) MACI (kN.m) MÉD.: 0,98 D.P.: 0,09 C.V.: 9,5% R.C.S.:57,1%

y = 1.121x R² = 0.9455

0 20 40 60 80 100

0 20 40 60 80 100

M u ( kN .m) Mfib14 (kN.m) MÉD.: 1,20 D.P.: 0,28 C.V.: 23,3% R.C.S.: 24,5%

y = 1.2253x R² = 0.8646

0 50 100 150 200 250 300

0 50 100 150 200 250 300

M u ( kN .m) Mfib14 (kN.m) MÉD.: 1,18 D.P.: 0,36 C.V.: 30,4% R.C.S.: 37,1%

y = 1.0656x R² = 0.9631

0 20 40 60 80 100

0 20 40 60 80 100

M u ( kN .m) Mfib14 (kN.m) MÉD.: 1,04 D.P.: 0,15 C.V.: 14,4% R.C.S.: 35,7% 67 106 0 20 40 60 80 100 120

ACI 440.2R fib14

**P**

**en**

**al**

**ties**

ACI 440.2R fib14

<0,5 0% 0%

0,5-0,65 0% 1%

0,65-0,85 2% 12%

0,85-1,15 52% 36%

1,15-2 44% 47%

>2 2% 3%

Revista ALCONPAT, 9 (1), 2019: 30 – 47

a) ACI 440-2R (2008) b) *fib Bulletin 14 (2001) *

Figure 12. Influence of the number of strengthening layers.

Figure 13 shows the influence of the proportion between the reinforcement ratio after the strengthening and the flexural reinforcement ratio (ρr/ρ). There is a trend of less conservative results

as ρr / ρ increases, and for values above 1.4, ACI tends to stabilize this trend, avoiding estimates
of strength against safety. However, the same was not observed for *fib 14, whose predictions *
approached the dashed line, which expresses the limit of the design strength.

a) ACI 440-2R (2008) b) *fib Bulletin 14 (2001) *

Figure 13. Influence of the reinforcement ratio increase (ρr/ρ)

Figures 12 and 13 show that the number of layers of CFRP is not necessarily a parameter that
should be penalized in the prediction of strength of flexural reinforced beams with sheets of CFRP
as defined by the ACI. This is evident from, for example, the results of Beber et al. (2000), who
tested beams with up to ten layers of CFRP sheets and obtained good performance, and those of
Bilota et al. (2015), whose beams tested had only one or two layers of CFRP and showed much
lower performance. By analyzing Figure 13, the beams of Beber et al. (2000) present low values
of *ρ*r/ρ while those of Bilota *et al. (2015) presented extreme values within the beams of this *

0.0 0.5 1.0 1.5 2.0 2.5

0 1 2 3 4 5 6 7 8 9 10

Layers
*M*_{u }/ *M*_{ACI}

Beber *et al.*(2000)

Bilota *et al.*(2015)

0.0 0.5 1.0 1.5 2.0 2.5

0 1 2 3 4 5 6 7 8 9 10

Layers

*M*u/ *Mfib*14

Beber *et al.*(2000)

Bilota *et al.*(2015)

0.0 0.5 1.0 1.5 2.0 2.5

1 1.2 1.4 1.6 1.8

rr/r

*M*u/ *M*ACI

Beber *et al.*(2000)

Bilota *et al.*(2015)

0.0 0.5 1.0 1.5 2.0 2.5

1 1.2 1.4 1.6 1.8

rr/r

*M*u/ *M*fib14

Beber *et al.*(2000)

Revista ALCONPAT, 9 (1), 2019: 30 – 47

database, evidencing that *ρ*r/ρ is a fundamental parameter to be taken into consideration in the

design.

**5.**

**CONCLUSION **

In order to observe the influence of reinforcement anchorage with CFRP on the behavior of beams resisting to flexure, an experimental study was carried out, involving tests on 4 reinforced concrete beams, varying the anchorage criteria of the carbon fiber sheets. In addition to the experimental approach, a database with results from several authors was used to evaluate the influence of different parameters on the strength of reinforced beams to flexion with CFRP sheets. These data were also used to discuss the performance of the theoretical methods proposed by fib Bulletin 14 (2001) and ACI 440-2R (2008).

As for beam tests, it was observed that the clamping width had a greater influence on the flexural strength of the reinforced beams with CFRP sheet, since the V4 beam presented the greatest strength in relation to the others, even though the anchoring length was identical to the one of the beam V3. The beams V2 and V3 presented the same values of strength, although the beam V3 presented a greater length of anchorage between them. Another important point is that, even with the strength additions of the reinforced beams in relation to the reference, the beams with CFRP sheet have failed prematurely. Finally, it was observed that the limit values of strain of the CFRP sheet assumed by the manufacturer are very conservative in face of the experimental results recorded in this research.

As for the evaluation of the theoretical models, it is verified that both the *fib 14 and the ACI *
presented conservative results in relation to the Mu/MRteo ratio, which in practice should guarantee

predictions of strength in favor of safety in most cases. It was also observed that the procedure of reducing reinforcement efficiency by means of limitations on CFRP strains, although generally in favor of safety, may become excessively conservative in cases of reinforcement where CFRP anchorage is performed properly. Finally, it is emphasized that among the evaluated parameters that affect the flexural strength of beams with CFRP sheets, it is worth noting that the ratio ρr/ρ was

more relevant than the number of layers of CFRP sheets, considering the data of this database.

**6.**

**ACKNOWLEDGMENTS **

For the support on this and other researches, the authors thank: the Federal University of Pará (UFPA); to the Nucleus of Amazonian Development in Engineering (NDAE); to the Nucleus of Applied Structural Modeling (NUMEA); to the University Campus of Tucuruí (CAMTUC); to Eletrobras Eletronorte; to VIAPOL Ltda for donating the reinforcement material used in the experiments; and the development agencies CNPq, CAPES and FAPESPA.

**7.**

**REFERENCES **

Alagusundaramoothy, I., Harik, I. E., Choo, C. C. (2003), *Flexural Behavior of R/C Beams *
*Strengthened with Carbon Fiber Reinforced Polymer Sheets or Fabric. *ASCE - Journal of
Composites for Constructions. 7 (4):292-301.
https://doi.org/10.1061/(ASCE)1090-0268(2003)7:4(292)

American Concrete Institute. (2014), *ACI Committee 318-M. Building Code Requirements for *
*Structural Concrete and Commentary. Farmington Hills, Michigan. *

Revista ALCONPAT, 9 (1), 2019: 30 – 47

Balaguru, P., Kurtz, S. (2001), Comparison of inorganic and organic matrices for strengthening
*of RC beams with carbon sheets. Journal of Structural Engineering, 127:35-42. *

Barros, J. A. O., Dias, S. J. E., Lima, J. L. T. (2007), Efficacy of CFRP-based techniques for the
*flexural and shear strengthening of concrete beams. Cementand Concrete Composites. Volume 29, *
Issue 3, Pages 203-217. https://doi.org/10.1016/j.cemconcomp.2006.09.001

Beber, A. J. (2003), “Comportamento Estrutural de Vigas de Concreto Armado Reforçadas com
* Compósitos de Fibra de Carbono”. Tese de Doutorado, Universidade Federal do Rio Grande do *
Sul, p. 289.

Beber, J. A., Campos Filho, A., Campagnolo, J. L. (2000), “Estudo Teórico-Experimental de Vigas
*de Concreto Reforçadas com Tecidos de Fibra de Carbono”. IV Simpósio EPUSP sobre estruturas *
de concreto, São Paulo.

Benjeddou, O., Ouezdou, M. B., Bedday, A. (2007), Damaged RC beams repaired by bonding of
*CFRP laminates. *Construction and Building Materials. Volume 21, Issue 6, Pages 1301-1310.

https://doi.org/10.1016/j.conbuildmat.2006.01.008

Bilotta, A., Ceroni, F., Nigro, E., Pecce, M. (2015), Efficiency of CFRP NSM strips and EBR plates
*for flexural strengthening of RC beams and loading pattern influence. Composite Structures, *
124:163-175. http://dx.doi.org/10.1016/j.compstruct.2014.12.046

Breña, S. F., Bramblett, R. M., Wood, S. L., Kreger, M. E. (2003), Increasing Flexural Capacity
* of Reinforced Concrete Beams Using Carbon Fiber-Reinforced Polymer Composites. *ACI
Structural Journal. 100:36-46.

Chahrour, A., Soudki, K. (2005), Flexural Response of Reinforced Concrete Beams Strengthened
*with End-Anchored Partially Bonded Carbon Fiber-Reinforced Polymer Strips. ASCE Journal of *
Composites for Construction. 9 (2):170-177.
https://doi.org/10.1061/(ASCE)1090-0268(2005)9:2(170)

Collins, M. P. (2001), “Evaluation of shear design procedures for concrete structures”. A Report prepared for the CSA technical committee on reinforced concrete design.

David, E., Ragneau, E., Buyle-Bodin, F. (2003), *Experimental analysis of flexural behavior of *
*externally bonded CFRP reinforced concrete structures. RILEM Materials and Structures. *
38:238-241.

Dias, S. J. E., Juvandes, L. F. P., Figueiras, J. A. (2002), Comportamento de Vigas de Betão Armado
*Reforçadas à Flexão com Sistemas Compósitos de CFRP. Unidireccionais. Engenharia Civil UM. *
14:15-28.

Dong, J. F., Wang, Q. Y., Qiu, C. C., He, D. (2011), *Experimental study on RC *
*beams strengthened with CFRP sheets. Advanced Materials Research. 213:548-52. *

Dong, J. F., Wang, Q. Y., Zhu, Y. M., Qiu, C. C. (2010), *Experimental study on RC beams *
*strengthened with externally bonded FRP sheets. *Journal of Sichuan University (Engineering
Science Edition). 42:197-203.

Esfahani, M. R., Kianoush, M. R., Tajari, A. R. (2007), Flexural behavior of reinforced concrete
*beams * *strengthened * *by * *CFRP * *sheets. * Engineering Structures. 29:2428-2444.

10.1016/j.engstruct.2006.12.008

Eurocode 2 (2004), *Design of Concrete Structures—Part 1-1: General Rules and Rules for *
*Buildings. Brussels, Belgium. *

Ferrari, V. J. (2007), “Reforço à Flexão de Vigas de Concreto Armado com Manta de Polímero
*Reforçado com Fibras de Carbono (PRFC) Aderido a Substrato de Transição Constituído por *
*Compósito Cimentício de Alto Desempenho”. Tese de Doutorado, Escola de Engenharia de São *
Carlos da Universidade de São Paulo, p. 310.

Revista ALCONPAT, 9 (1), 2019: 30 – 47

Garcez, M. R. (2007), “Alternativas para Melhoria no Desempenho de Estruturas de Concreto
*Armado Reforçadas pela Colagem de Polímeros Reforçados com Fibras”. Tese de Doutorado, *
Universidade Federal do Rio Grande do Sul, p. 241.

Hawileh, R. A., Nawaz, W., Abdalla, J. A., Saqan, E. I. (2015), Effect of flexural CFRP sheets on
*shear strength of reinforced concrete beams. * Composite Structures. 122:468-476.

https://doi.org/10.1016/j.compstruct.2014.12.010

Juvandes, L. F. P. (1999), “Reforço e reabilitação de estruturas de betão usando materiais
*compósitos de “CFRP”. Tese de Doutorado, Faculdade de Engenharia da Universidade do Porto, *
p. 302.

Khan, A. R., Fareed, S. (2014), *Behaviour of reinforced concrete beams strengthened by CFRP *
*wraps * *with * *and * *without * *end * *anchorages. * Procedia Engineering. 77:123-130.

https://doi.org/10.1016/j.proeng.2014.07.011

Kim, H. S., Shin, Y. S. (2011), *Flexural behaviour of reinforced concrete *
*(RC) * *beams * *retrofitted * *with * *hybrid * *fiber * *reinforced * *polymers * *(FRPs) *
*under sustaining loads. Composite Structures. 93:802-11. *

Monti, G., Liotta, M. A. (2007). *Tests and design equations for FRP-Strengthning in shear. *

Construction and Building Materials. 21:799-809.

https://doi.org/10.1016/j.conbuildmat.2006.06.023

Rafi, M. M., Nadjai, A., Ali, F., Talamona, D. (2008), Aspects of behavior of CFRP reinforced
*concrete * *beams * *in * *bending. * Construction and Building Materials. 22:277-285.

https://doi.org/10.1016/j.conbuildmat.2006.08.014

Rusinowsky, P., Taljsten, B., Sand, B. (2009), “Peeling Failure at the Cut-off End of CFRP
* Strengthened RC Beams”. Proceedings of the 9*th

_{ International Symposium of the Fiber-Reinforced }

Polymer Reinforcement for Reinforced Concrete Structures, Sydney.

Spadea, G., Bencardino, F., Swamy, R. N. (2000), Optimizing the performance characteristics of
*beams strengthened with bonded CFRP laminates. Materials and Structures. 33:119-126. *

Teng, J. G., Smith, S. T., Yao, J., Chen, J. F. (2003), Intermediate crack-induced debonding in RC
*beams and slabs. Construction and Building Materials. 17:447-462. *
10.1016/S0950-0618(03)00043-6

Toutanji, H., Zhao, L., Zhang, Y. (2006), *Flexural behavior of reinforced concrete beams *
*strengthened with CFRP sheets bonded with an inorganic matrix. Engineering Structures, *
28:557-566. 10.1016/j.engstruct.2005.09.011

Vieira, M. M., Santos, A. R. S., Mont’Alverne, A. M., Bezerra, L. M., Montenegro, L. C. S. and
Cabral, A. E. B. (2016), *Experimental analysis of reinforced concrete beams strengthened in *
*bending with carbon fiber reinforced polymer. IBRACON Structures and Materials Journal. 9 (1) *
pp. 123:152. http://dx.doi.org/10.1590/S1983-41952016000100008

Zhang, A., Jin, W., Li, G. (2006), Behavior of preloaded RC beams strengthened with CFRP
* laminates. * Journal of Zhejiang University SCIENCE A. 7:436-444.